ISSN Print: 2327-4077
DOI: 10.4236/jmmce.2018.65039 Aug. 31, 2018 541 J. Minerals and Materials Characterization and Engineering
Review of GTAW Welding Parameters
Bolarinwa Johnson Kutelu1
, Saliu Ojo Seidu2
, Godwin Idenala Eghabor2
Ayotunde Idris Ibitoye2
1Department of Minerals and Petroleum Resources Engineering, Federal Polytechnic, Ado Ekiti, Nigeria 2Department of Metallurgical and Materials Engineering, Federal University of Technology, Akure, Nigeria
Welding as a fabrication process is one of the vital production routes for most manufacturing industries. Several factors are involved in the choice of weld-ing process for specific applications; notable among these are compositional range of the material to be welded, the thickness of the base materials and type of current. Most metals oxidize rapidly in their molten state, and there-fore, the weld area needs to be protected from atmospheric contamination; this is achieved in gas tungsten arc welding GTAW by a shielding gas (argon, helium, nitrogen). GTAW technique is one of the major processes for joining austenitic stainless steels (ASS) and ferritic stainless steel (FSS) fabrication. However, the microstructural change that occurs during welding and at weld joint is still a major challenge today as it affects both the corrosion resistance and the mechanical properties. Therefore, this present paper reviews past re-search findings on GTA welding of ASS and FSS. Results of the findings have confirmed that, depending on the amount of heat input, which can be con-trolled by welding parameters (welding speed, voltage and current), welded joints particularly, heat affected zones (HAZs) of both grades of steels can undergo mechanical failure and can be susceptible to corrosion attack if the joints are produced with a less ideal combination of welding parameters.
Austenitic Stainless Steel (ASS), GTA Welding, Heat Affected Zone (HAZ), Welding Speed, Voltage, Current, Heat Input, Shielding Gas, Filler Metal
Welding is a process involving the joining of two crystalline work pieces usually of metal by bringing their fitted surfaces into such intimate contact that crys-tal-to-crystal bonding occurs. Depending on the welding techniques, heat
re-How to cite this paper: Kutelu, B.J., Seidu, S.O., Eghabor, G.I. and Ibitoye, A.I. (2018) Review of GTAW Welding Parameters. Journal of Minerals and Materials Charac-terization and Engineering, 6, 541-554.
Received: March 27, 2018 Accepted: August 28, 2018 Published: August 31, 2018
Copyright © 2018 by authors and Scientific Research Publishing Inc. This work is licensed under the Creative Commons Attribution International License (CC BY 4.0).
DOI: 10.4236/jmmce.2018.65039 542 J. Minerals and Materials Characterization and Engineering quired for welding can be obtained from a burning gas or an electric arc, or gen-erated by electric resistance . The fitted surfaces may melt together, or a filler rod may melt between them to form a connecting bridge. Area of industrial ap-plications is seen in buildings, bridges, ships, pressure vessels and nuclear reac-tors among others . The increasing use of welding in these areas is predicated upon its many advantages such as design flexibility, economy (cost savings), re-duced overall weight and enhanced structural performance  . Based on the heat source, fusion welding is divided into gas, arc and high-energy beam weld-ing. In arc welding, energy is transferred from the welding electrode to the base metal by an electric arc; upon starting the arc, a sufficient amount of power (energy transferred per unit time) and energy density is supplied to the elec-trode. Both the base metal and the filler metal are melted to create the weld  .
Gas Tungsten Arc Welding (GTAW) also referred to as Tungsten Inert Gas (TIG) uses a non-consumable tungsten electrode to produce the weld. Under the correct welding conditions, the tungsten electrode does not melt. It operates by creating an electric arc between the tungsten electrode and the work piece; the electric arc can produce temperatures of up to 19,400˚C . In GTAW, weld can be made with or without filler metal. When filler metal is used, it is added di-rectly into the molten pool by dipping the end of a filler rod into the leading edge of the molten weld pool, when filler metal is not used, edges of the metal are heated, melted and flowed together by themselves, and as the molten metal cools, coalescence occurs and the parts are joined, resulting in weld requiring minimum finishing  . The common use of GTAW as components assem-bling technique has been linked to its high quality welds, which is attributable to high degree of control of heat input and filler additions. GTAW has found wide appreciation in areas where precision welding is required, notable among which included atomic energy, aircraft, chemical and instrument industries, nuclear industry, food industry, maintenance and repair work and some manufacturing areas . Also, GTA welding is widely utilized for the joining of high strength, reactive metals and alloys such as stainless steel, aluminium and magnesium al-loys  . In addition, copper, brass, titanium, nickel and nickel alloys, stainless steel, inconel, high temperature and hard surfacing alloys like zirco-nium, titanium have been successfully welded with the GTA welding techniques .
(cur-DOI: 10.4236/jmmce.2018.65039 543 J. Minerals and Materials Characterization and Engineering rent, voltage, speed etc.), geometric shape, design of the welding piece, the me-thod implemented for welding and the nature of the applied stresses and others . Low productivity, relative shallow penetration and high sensitivity of the surface condition and chemical composition of the base metal are some of the disadvantages associated with GTAW process .
1.1. Primary GTAW Process Parameters1.1.1. Welding Current
Welding current is the most influential variable in arc welding process which controls the electrode burn off rate, the depth of fusion and geometry of the weldments. Current has direct influence on weld bead shape, on welding speed and quality of the weld. Most GTAW welds employ direct current on electrode negative (DCEN) (straight polarity) because it produces higher weld penetration depth and higher travel speed than on electrode positive (DCEP) (reverse polar-ity). Besides, reverse polarity produces rapid heating and degradation of the electrode tip, because anode is more heated than cathode in gas tungsten electric arc. Higher current in GTA welding can lead to splatter and work piece become damage. Again lower current setting in GTA welding lead to sticking of the filler wire. Sometimes larger heat affected area can be found for lower welding cur-rent, as high temperatures need to applied for longer periods of time to deposit the same amount of filling materials. Fixed current mode will vary the voltage in order to maintain a constant arc current  .
1.1.2. Welding Voltage
This is the electrical potential difference between the tip of the welding wire and the surface of the molten weld pool. Welding voltage can be fixed or adjustable depending on the GTA welding equipment. It determines the shape of the fusion zone and weld reinforcement. A high initial voltage allows for easy arc initiation and a greater range of working tip distance. However, it produces wider, flatter and less deeply penetrating welds than low welding voltages, depth of penetra-tion is maximum at optimum arc voltage, to high voltage on the other hand will lead to large variable in welding quality .
1.1.3. Welding Speed
DOI: 10.4236/jmmce.2018.65039 544 J. Minerals and Materials Characterization and Engineering of melted material. Normal welding speeds are from 100 to 500 mm/min de-pending on current, material type and plate thickness .
1.1.4. Heat Input
Heat input is a relative measure of the energy transferred per unit length of weld. The higher the heat input, the slower the cooling rate. Conversely, the lower the heat input, the faster the cooling rate. Hence, like preheat and interpass temper-ature, heat input is an important characteristic that influences the cooling rate, which may affect the mechanical properties and metallurgical structure of the weld and the HAZ . In arc welding, it is well known that energy is trans-ferred from the welding electrode to the base metal by an electric arc. Upon starting the arc, sufficient amount of power (energy transferred per unit time) and energy density is supplied to the electrode. Consequently, both the base metal and the filler metal are melted to create the weld  . Heat input is typically calculated as the ratio of the power (i.e., voltage × current) to the veloc-ity of the heat source (i.e., the arc). Heat input was calculated according to equa-tion 1
where, H = heat input in KJ/mm, η = efficiency = 0.60 for GTAW, V = voltage in volts,
I = current in amperes, ν = welding speed in mm/sec.
1.1.5. Shielding Gases
Shielding gases are used in GTAW in order to prevent atmospheric contamina-tion of the weld metal. This contaminacontamina-tion can produce porosity, weld cracking, scaling and even change in the chemical composition of melted material. Besides shielding gas also has a large influence on the stability of the electric arc. Gases with low ionization potential facilitate the ignition of the electric arc and those with low thermal conductivity tend to increase the arc stability. Argon is the most used GTAW shielding gas. It has low ionization potential and is heavier than air, providing an excellent shielding of the molten weld pool. Furthermore it is less expensive than helium, the other inert shielding gas used in the process. Argon is used in welding of carbon and stainless steels and low thickness alu-minum alloys components. For welding thick alualu-minum work-pieces and other high-conductive materials, such as copper alloys, helium is recommended be-cause it has higher ionization potential than argon, needing higher voltage for
arc initiation and maintenance, but producing higher heat-input  . The
DOI: 10.4236/jmmce.2018.65039 545 J. Minerals and Materials Characterization and Engineering Helium or helium/argon (30% - 80% He) mixtures allow increased welding speed and improved process tolerance. Mixtures of argon with up to 5% of hy-drogen are frequently used in welding of austenitic stainless steels. Hyhy-drogen increases arc-voltage and consequently heat input, increasing weld penetration and weld travel speed, as well as improving weld appearance . Ar-gon/hydrogen mixtures are also used in welding of copper nickel alloys. Argon is also used as back side shielding gas, mainly in welding of stainless steels, alumi-num alloys and reactive metals. Flow rates of shielding gases depend on weld thickness, being 4 - 10 l/min for argon and 10 - 15 l/min for helium, because it is lighter than argon, and consequently less effective in shielding purposes . Gases with a purity of 99.995% are used in welding most of the metals, though reactive materials such as titanium need contaminant level less than 50 ppm. The choice of shielding gas is very important as it affects weld penetration depth and surface profile, porosity, corrosion resistance, strength, hardness and brit-tleness of the weld material  .
The choice of shielding gas dependent on the working metals and effects on the welding cost, weld temperature, arc stability, weld speed, splatter and elec-trode life. Argon or Helium may be used successfully for GTA welding applica-tions. For welding of extremely thin material pure argon is used. Argon general-ly provides an arc which operates more smoothgeneral-ly and quietgeneral-ly. Penetration of arc is less when Argon is used than the arc obtained by the use of Helium. For these reasons argon is preferred for most of the applications, except where higher heat and penetration is required for welding metals of high heat conductivity in
larg-er thicknesses   . Argon hydrogen mixture is used for welding of
some grades of stainless steels and nickel alloys. Pure helium may be used for aluminium and copper. Helium argon mixtures may be used for low alloy steels, aluminium and copper .
1.1.6. Filler Metal
DOI: 10.4236/jmmce.2018.65039 546 J. Minerals and Materials Characterization and Engineering that welds are slightly ferromagnetic. Those alloys that solidify fully or nearly fully austenitic must be welded with lower heat inputs. For certain applications, a low ferrite weld metal is desirable, and certain filler metals are produced for that purpose. For most 300 series stainless steels, a nominally matching filler metal is the most common filler metal used  .
2. Literature Review
 investigated inert gas tungsten arc welding parameters on the mechanical properties of SS 316 L weldments. 316 ASS rods of dimensions of 25 mm diame-ter and 75 mm length were used. Current, bevel angles gas volumes inputs were varied at different range of 90, 100 and 110 ampere, 60˚ 70˚ and 80˚ and 1.1, 0.9, 0.71 per litre respectively. Taguchi L-9 orthogonal array technique was used. Results obtained showed that the current of 110 A, bevel Angle of 60˚ and a gas flow of 0.7 l pm offers the maximum tensile strength. While the minimum ten-sile strength was obtained with current of 100 A, bevel Angle of 60˚ and a gas flow of 0.9 per litre. In addition, sample with the minimum tensile strength gave the maximum micro hardness. They concluded that, as micro hardness increas-es, tensile strength decreases.
Influence of welding speeds and power inputs on the heat affected zone (HAZ) microstructural characteristics and tensile behaviour of type 304 L auste-nitic stainless steel was studied by . The butt joint HAZ square geometry samples were produced using Gas Metal Arc Welding (GTAW) process. Results obtained showed that the microstructures were composed mainly of mixture of austenite and ferrite phases. Variations in volume fraction and grain size of the phases were observed at the different welding speeds and power inputs. Chro-mium carbide formation and precipitation due to sensitization was seen at the grain boundaries. Optimum ultimate tensile strength (UTS) and yield strength (YS) were obtained for HAZ sample at moderate (4.5 mm/s) welding speed, and optimum % elongation at slow welding speed, and optimum UTS and YS were obtained for HAZ sample at power input of 9.2 KW, and optimum % elongation at 12.00 KW. Influence of the welding variables on tensile characteristics in the HAZ was found substantial.  investigated the effect of GTA welding current, gas flow rate, thickness of work piece on the bead geometry of AISI 304 L, and reported all the process parameters exhibited high influence on the mechanical properties of the material.
al-DOI: 10.4236/jmmce.2018.65039 547 J. Minerals and Materials Characterization and Engineering ternate supply of shielding gases on austenite stainless steel GTA welded 304 SS. To this end, both conventional and alternate methods were used. Specimen of 200 lengths, 100 weights and 12 thicknesses was used, and the input parameters used were shielding gas, welding current and welding voltage. Under similar welding conditions, the results obtained revealed that the alternate method with Ar and He, produced the lowest degree of welding distortion as compared to the conventional methods of Ar and Ar + 67% He. Hence, the alternate method has the possibility of solving the problem of the increase in gas cost and welding distortion.
 investigated the effect of TIG pulse rate, pulse frequency, arc travel speed and wire feed rate on tensile and hardness properties of girth welding of SS 304 L. The pipes were welded by using orbital welding machine, ER 308 L filler wire was used for reinforcement of weld. Results obtained showed that sample welded with 90 A pulse current revealed superior tensile strength and hardness proper-ties. Tensile property of 605 MPa, and hardness values of the base metal, HAZ and weld metal were 160 HB, 114 HB and 99 HB respectively. With increasing pulse current, tensile strength and soundness of joint was observed to increase, maximum strength of the joint was obtained at 2.5 Hz frequency. And at the arc travel speed of 80 mm/min, maximum strength and soundness of joint was ob-tained, but with increasing time for making the joint. Also, as the wire feed rate was increased without increase in current; the strength of joint was reported to decrease.
 revealed that welding process relies on an intensely localized heat input, which tends to generate undesired residual stresses and deformations in welded structures, especially in the case of thin plates. Increasing the speed of travel and maintaining constant arc voltage and current will reduce the width of bead and also increase penetration until an optimum speed is reached at which penetra-tion will be maximum. Increasing the speed beyond this optimum will result in decreasing penetration  . Increase in welding speed causes 1) decrease in the heat input per unit length of the weld, 2) decrease in the electrode burn off rate, and 3) decrease in the weld reinforcement  . Excessive high welding speed decreases wetting action, increases tendency of undercut, porosity and uneven bead shapes and Slower welding speed reduces the tendency to porosity. If the welding speed decreases beyond a certain point, the penetration also will decrease due to the pressure of the large amount of weld pool beneath the elec-trode, which will cushion the arc penetrating force . With increasing welding speed, power or heat input per unit length of weld decreases with attendant less weld reinforcement and decreased penetration, and with excessive high welding speed, wetting action decreases with increasing tendency of undercut, porosity and uneven bead shapes, slower welding speed reduces the tendency to porosity .
DOI: 10.4236/jmmce.2018.65039 548 J. Minerals and Materials Characterization and Engineering argon environment at a heat flux between 1008 W to 1584 W and speed between 2.5 mm/s and 3.5 mm/s. The width of the sensitization zone increases with in-creasing the heat input. The depth of the sensitization zone in the thickness di-rection is insignificant and it is generally within one half of a millimetre. The use of heat input greater than 432 J/mm increases the development of sensitized re-gions. This level of heat input corresponds to heat fluxes in the range 1008 - 1296 W and welding speed between 3 mm/s and 3.5 mm/s. Under this condition the average cooling time is about 10 s. Most grain attack is restricted to the fer-rite-ferrite grain boundaries. The ferrite martensite boundaries do not show vis-ible attack. This indicates that welding condition that promotes the formation of martensite in the HAZ is ideal for the presentation of sensitization.
 investigated the effects of welding speeds on the hardness property of type 304 L austenitic stainless steel heat affected zone (HAZ). Thirty samples were produced, and welded under a range of welding variables to produce butt joint HAZ samples. They reported that hardness property of the HAZ was in-fluenced at varying degrees by the range of welding speeds and power inputs. Optimum hardness property was obtained at fast welding speed of 9.5 m/min and 9.20 kW power input.  investigated the effect of various welding para-meters on the penetration of GTA welds. Increases in welding speed were found to reduce penetration; however, increases in welding current were observed to increase the penetration in high sulfur (HS) casts and decrease penetration in low sulfur (LS) steels. It was also observed that penetration as a function of in-creasing linear energy (the heat supplied per unit length of weld) revealed a sim-ilar trend with increased penetration in HS casts, but the penetration in LS casts was unaffected by increases in linear energy. Their results support the Bur-gardt-Heiple proposition that changes in welding parameters on penetration can be explained in terms of their effect, sequentially, on the temperature gradient and the Marangoni forces operating in the weld pool. Increases in arc length were found to decrease weld penetration regardless of the sulfur concentration of the steel, and the effects of electrode geometry and welding position on weld penetration.
DOI: 10.4236/jmmce.2018.65039 549 J. Minerals and Materials Characterization and Engineering and maintaining all parameters constant hardness, impact and tensile strength of the welded joints are tested and finally, microstructure details are analyzed. The results showed mechanical properties linearly varies with increase in weld cur-rent.
The effect of heat input, inter-pass temperature, cooling rate, shielding/back purging gas, on corrosion behavior was studied by . DSS and SDSS pipes were welded with Gas Tungsten Arc Welding (GTAW) process. In order to en-sure that no flaw was present in the weld, test samples were subjected to non-destructive testing and were prepared for microstructural examinations and ferrite content measurements. And the test samples were subjected to corrosion tests. ASTM G48 test standard was used for the determination of pitting corro-sion rate. Potentiodynamic polarization tests and potentiostatic tests were used to verify susceptibility of the alloys to corrosion attack. From the results ob-tained, they observed that the complex microstructure of root region may have resulted from the repetitive heating of the zone during different weld layers. They reported that desirable microstructure was formed at low heat input. And from the corrosion behaviour results, they reported that DSS weldments had CPT in between 23˚C to 27˚C and SDSS weldments had CPT between 37˚C to 41˚C in potentiostatic measurements. The corrosion test results were correlated to the microstructures of the weldments, and the pitting resistance of individual phases was studied and the effect of secondary austenite on corrosion attack was also observed.
Microstructure and mechanical properties of AISI 304 austenitic stainless steels welded by GTA welding was studied by . 308 grade filler metal was used. Microstructures of base metal, heat affected zone and fusion zone were studied with microscopy. Result obtained in the heat affected zone and fusion zone revealed presence of chromium carbide precipitates and dendrite structure, which was reported to have resulted from sensitisation, this finding confirms further that due to sensitisation, unstabilised austenitic stainless steels are cha-racterised by precipitation of a network of chromium carbides.
 examined effect of welding current and filler metal types on the percent elongation of 3 mm thick austenitic steel (304L grade) welded joint. They consi-dered five welding currents in the range of 91 - 95 amperes at 1 ampere interval, and used three types of filler metal namely ER308L, ER309L and ER316Ld to produce square butt weld joints. Standard equipment and ASTM standard pro-cedure were used for determining percent elongation. And reported based on results obtained that percent elongation for all filler metal types increased with increase in welding current, but were generally lower than that of the base metal.
DOI: 10.4236/jmmce.2018.65039 550 J. Minerals and Materials Characterization and Engineering process shifted the corrosion potential values to more anodic potentials. And due to welding effect, corrosion current densities and the passive current densi-ties were also observed to increase with increasing temperature. Also, they ob-served that as a result of passivation of material, open circuit potential values were located in the passive zone of the potentiodynamic curves. They reported that galvanic corrosion of the pair was not severe in the studied conditions. The ratio between the galvanic current density of the pair and the corrosion current density of the uncoupled anode was reported to be less than 5, an implication of compatibility of the members in the couple.
Based on the review, the following conclusions are drawn:
1) Welding parameters have influence on the mechanical properties (tensile, hardness, impact) of GTA welded joints;
2) Corrosion behaviours of GTA welded joints are influenced by welding pa-rameters in varied degrees;
3) High quality GTA welded joint depends primarily on optimized welding parameters arrangement.
Better economy, improved efficiency and high profitability are some notable derivable advantages obtainable through proper welding input parameters selec-tion.
Conflicts of Interest
The authors declare no conflicts of interest regarding the publication of this pa-per.
 Benjamin, W.N., Alan, B.D. and Richard, A.W. (1989) Modern Manufacturing Process Engineering. McGraw-Hill College, 627-628.
 Ramesh, K.N. and Chauhan, P.M.R. (2014) Mechanical Properties and Microstruc-tural Investigations of TIG Welded 40 mm and 60 mm Thick SS 316L Samples for Fusion Reactor Vacuum Vessel Applications. Fusion Engineering and Design, 89, 3149-3158. https://doi.org/10.1016/j.fusengdes.2014.10.006
 Dutta, J. and Narendranath, S. (2014) Estimation of Cooling Rate and Its Effect on Temperature Dependent Properties in GTA Welded High Carbon Steel Joints,
Welding Journal, 10, 149-155.
 Lee, W.-S., Tzeng, F.-T. and Lin, C.-F. (2005) Mechanical Properties of 304L Stain-less Steel SMAW Joints under Dynamic Impact Loading. Journal of Materials Science, 40, 439-484.https://doi.org/10.1007/s10853-005-1920-0
 Ghosh, A and Mallik, A.K. (2008) Manufacturing Science. East-West Press Private Limited, New Delhi, 63-68.
DOI: 10.4236/jmmce.2018.65039 551 J. Minerals and Materials Characterization and Engineering https://doi.org/10.1016/j.matdes.2013.03.029
 Arpita, N.B. and Vikram, A.P. (2016) Influence of Process Parameters of TIG Welding Process on Mechanical Properties of 304LSS Welded Joint. International Research Journal of Engineering and Technology, 3, 977.
 Lokesh, K.G., Karthikeyan, P., Narasimma, R.C., Prasanna, B. and George, O. (2015) Microstructure and Mechanical Properties of ASS (304)-FSS (430) Dissimilar Joints in IN SMAW and GTAW Process. International Journal of Engineering Sciences and Research Technology, 6, 367-378.
 Kumar, A. and Sundarrajan, S. (2009) Effect of Welding Parameters on Mechanical Properties and Optimization of Pulsed TIG Welding of Al-Mg-Si Alloy. Advanced Manufacturing Technology, 42, 118-125.
 Subodh, K. and Shahi, A.S. (2011) Effect of Heat Input on the Microstructure and Mechanical Properties of Gas Tungsten Arc Welded AISI 304 Stainless Steel Joints,
Materials and Design, 32, 3617-3623. https://doi.org/10.1016/j.matdes.2011.02.017  Sindo, K. (2003) Welding Metallurgy. 2nd Edition, Wiley, Hoboken.
 Munoza, A.C., Ruckert, G., Huneau, B., Sauvage, X. and Marya, S. (2008) Compari-son of TIG Welded and Friction Stir Welded Al-4.5Mg-0.26Sc Alloy. Journal of Materials Processing Technology, 197, 337-343.
 Lakshman, S., Rohit, K., Nidhi, G. and Mayur, G. (2013) Investigating the Effect of TIG Welding Parameters 5083 Aluminium Alloy Weldability. Materials and Design, 2, 37-44.
 Ahmet, D. (2004) Experimental Investigation of the Effect of Hydrogen in Argon as a Shielding Gas on TIG Welding of Austenitic Stainless Steel. Materials and Design, 25, 19-23. https://doi.org/10.1016/j.matdes.2003.07.004
 Medvedv, S.V. (2002) Computer Modeling of Residual Welding Strains in Tech-nological Design of Welded Structures. Welding International, 16, 59-65.
 Salleh, M.S. (2011) Study on Mechanical Properties and Microstructure Analysis of AISI 304L Stainless Steel Weldments. Journal of Mechanical Engineering Technol-ogy, 3, 71-82.
 Seo, D.W., Jeon, Y.B. and Lim, J.K. (2003) Effect of Electric Weld Current on Spat-ter Reduction in Spot Welding Process. Key Engineering Materials, 261-263, 1623-1628.
 Atma, R.M.R. and Joy, V.V.M. (2014) Determination of Distortion Development during TIG Welding of Low Carbon Steel Plate. International Journal of Engineer-ing Research, 1, 23-29.
 Tewari, S.P., Gupta, A. and Prakash, J. (2010) Effect of Welding Parameters on the Weldability of Materials. International Journal of Engineering Science and Tech-nology, 2, 512-516.
 Abioye, T.E. (2017) The Effect of Heat Input on the Mechanical and Corrosion Properties of AISI 304 Electric Arc Weldments. British Journal of Applied Science and Technology, 20, 1-10. http://www.sciencedomain.org
DOI: 10.4236/jmmce.2018.65039 552 J. Minerals and Materials Characterization and Engineering
 Janunkar, R.G., Allurkar, S. and Mahesh, P. (2017) An Influence on Effect of Weld-ing Speed on Strength of Welded Joint UsWeld-ing Tig WeldWeld-ing Process. World Journal of Technology, Engineering and Research, 2, 337-342.
 Yuri, T., Ogata, T., Saito, M. and Hirayama, Y. (2000) Effect of Welding Structure and δ-Ferrite on Fatigue Properties for TIG Welded Austenitic Stainless Steels at Cryogenic Temperatures. Cryrogenics, 40, 251-259.
 Apurv, C. and Vijaykumar, S.J. (2014) Influence of Heat Input on Mechanical Properties and Microstructure of Austenitic 202 Grade Stainless Steel Weldments.
WSEAS Transactions on Applied and Theoretical Mechanics, 9, 222-228.
 Kang, B.Y., Yarlagadda, K.D., Prasad, V., Kang, M.J., Kim, H.J. and Kim, S. (2009) The Effect of Alternate Supply of Shielding Gases in a Austenite Stainless Steel GTA Welding. Journal of Materials Processing Technology, 209, 4722-4727.
 Sun, H., Song, G. and Zhang, L.F. (2008) Effects of Oxide Activating Flux on Laser Welding of Magnesium Alloy. Science and Technology of Welding and Joining, 13, 305-311.https://doi.org/10.1179/174329307X213846
 Ghazvinloo, H.R. and Honarbakhsh-Raouf, A. (2010) Effect of Gas Shielded Flux Cored Arc Welding Parameters on Weld Width and Tensile Properties of Weld Metal in Low Carbon Steel. Journal of Applied Science, 10, 658-663.
 Arun, N., Cijo, M., Vinod, Y.B. and Joby, J. (2013) Influence of Gas Tungsten Arc Welding Parameters on Aluminum 5083 Alloy. International Journal of Engineer-ing Science and Innovative Technology, 2, 113-118.
 Paniagua-Mercado, A.M., Lopez-Hireta, V.M., Mendez-Sanchez, A.F. and Sauce-do-Munoz, M.L. (2007) Effect of Active and Nonactive Fluxes on Mechanical Prop-erties and Microstructure in Sub-Merged-Arc Welds of A-36 Steel Plates. Journal of Materials and Manufacturing Processes, 223, 851-863.
 Qin, G.L., Wang, G.G. and Zou, Z.D. (2012) Effects of Activating Flux on CO2 Laser
Welding Process of 6013 Al Alloy. Transactions Nonferrous Metallurgical Society China, 22, 23-29.
 Bang, K.S., Jung, D.H., Park, C. and Chang, W.S. (2008) Effects of Welding Para-meters on Tensile Strength of Weld Metal in Flux Cored Welding. Science and Technology of Welding and Joining, 13, 508-514.
 Zhang, R., Fan, D. and Katayama, S. (2006) Electron Beam Welding with Activating Flux. Transactions of JWRI, 35, 19-12.
 Ibrahim, H. (2013) Study on Microstructure, Tensile Test and Hardness 304 Stain-less Steel Jointed by TIG Welding. International Journal of Science and Technology, 2, 23-34.
 Balaji, C., Abinesh, K.S.V., Ashwin, K.S. and Sathish, R. (2012) Evaluation of Me-chanical Properties of SS 316L Weldments Using Tungsten Inert Gas Welding. In-ternational Journal of Engineering Science and Technology, 4, 124-131.
 Oyetunji, A., Kutelu, B.J. and Akinola, A. (2013) Effects of Welding Speeds and Power Inputs on the Hardness Property of Type 304L Austenitic Stainless Steel Heat-Affected Zone (HAZ). Journal of Metallurgical Engineering, 2, 124.
DOI: 10.4236/jmmce.2018.65039 553 J. Minerals and Materials Characterization and Engineering
 Raveendra, S. (2012) Weldability and Process Parameter Optimization of Dissimilar Pipe Joints Using GTAW. International Journal of Engineering Research and Ap-plications, 2, 2525-2530.
 Ahmed, K.H., Abdul, L., Mohd, J. and Pramesh, T. (2010) Influence of Welding Speed on Tensile Strength of Welded Joint in TIG Welding Process. International Journal of Applied Engineering Research, 1, 518-527.
 Aamir, S., Abdul, A., Muhammad, I., Osama, J.M. and Sagheer, A. (2017) Effect of TIG Welding Parameters on the Properties of 304L Automated Girth Welded Pipes Using Orbital Welding Machine.
 Tsann-Shyi, C., Kuang-Hung, T. and Hsien-Lung, T. (2011) Study of the Characte-ristics of Duplex Stainless Steel Activated Tungsten Inert Gas Welds. Materials and Design, 32, 255-263.https://doi.org/10.1016/j.matdes.2010.05.056
 Iordachescu, M., Ruiz, H.J., Iordachescu, D., Valiente, A. and Caballero, L. (2010) Thermal Influence of Welding Process on Strength Overmatching of Thin Dissimi-liar Joints. Welding in the World, 65, 201-209.
 Muna, K.A., Jalal, M.J. and Abbas, S.A. (2009) Numerical and Experimental Ana-lyses for Effect Welding Currents on Cooling Rates in MMAW Process. Engineering and Technology Journals, 28, 2276.
 Tseng, K.H. and Hsu, C.Y. (2011) Performance of Activated TIG Process in Auste-nitic Stainless Steel Welds. Journal of Materials Processing Technology, 211, 503-512.https://doi.org/10.1016/j.jmatprotec.2010.11.003
 Devakumar, D. and Jabaraj, D.B. (2010) Research on Gas Tungsten Arc Welding of Stainless Steel—Overview. International Journal of Scientific and Engineering Re-search, 5, 39-54.
 Afolabi, A.S. (2008) Effect of Electric Arc Welding Parameters on Corrosion Beha-viour of Austenitic Stainless in Chloride Medium. AU Journal of Technology, 11, 171-180.
 Anuda, M.O.H. and Mridha, S. (2011) Analysis of Sensitization Profile in Medium Chromium Ferritic Stainless Steel (FSS) Welds. Journal of Integrated Engineering, 3, 17-22.
 Shirali, A.A. and Mills, K.C. (1993) The Effect of Welding Parameters on Penetra-tion in GTA, FoundaPenetra-tions of Material Science Engineering. McGraw Hill, New York, 78-98.
 Jaladi, D.S., Manne, V.R. and Srinivas, K. (2015) Analysis of TIG of TIG Welding Process on Mechanical Properties and Microstructure of Aa6063 Aluminium Alloy Joint. International Journal of Recent and Innovation Trends in Computing and Communication, 4, 623-626.
 Prabhu, P. and Rajnish, G. (2016) Effect of Welding Parameters on Pitting Behavior of GTAW of DSS and Super DSS Weldments.
 Kurt, H.I. and Samur, R. (2013) Study on Microstructure, Tensile Test and Hard-ness 304 Stainless Steel Jointed by TIG Welding. International Journal of Science and Technology, 2, 164-168.
 Okonji, P.O., Nnuka, E.E. and Odo, J.U. (2015) Effect of Welding Current and Filler Metal Types on Macrostructure and Tensile Strength of GTAW Welded Stainless Steel Joints. International Journal of Scientific Research and Engineering Trends, 1, 9-12.
DOI: 10.4236/jmmce.2018.65039 554 J. Minerals and Materials Characterization and Engineering